Anna Fischer,† Jens Oliver Mu¨ller,‡ Markus Antonietti,† and Arne Thomas†,* †
Max Planck Institute of Colloids and Interfaces, Research Campus Golm, Am Muehlenberg 1, D-14476 Golm, Germany, and ‡Fritz-Haber-Institute of the Max-PlanckSociety, Department of Inorganic Chemistry, Faradayweg 4-6, D-14195 Berlin, Germany
etal nitrides have attracted growing interest in recent years as their properties can complement metal oxides in a variety of applications. Thus, metal nitrides exhibit enhanced hardness and are therefore applied as abrasive materials.1 The metal nitrides formed from group III metals are wide band gap semiconductors and can be used as optoelectronic materials.2 Furthermore, the applications of metal nitrides as electrodes for supercapacitors3 or as catalyst4⫺8 were reported. Especially for the latter applications, the control of the nanostructure of the metal nitride and naturally its composition can have a crucial influence on its overall performance. In this respect, the formation of ternary metal nitrides, that is, of metal nitrides featuring two metals in their crystal structure, can widely expand the properties of this class of materials. This is especially obvious for the application of metal nitrides as semiconductors. The band gap of pure binary metal nitrides features values of 0.7 eV for indium nitride (InN), 3.4 eV for gallium nitride (GaN), and 6.3 eV for aluminum nitride (AlN), respectively, and thus can be used for violet, blue, and green light emitting devices.9 It is certainly appealing to mix such metal nitrides into ternary metal nitrides, as for example an Al⫺Ga⫺N alloy with different compositions will allow one to adjust the size of the band gap continuously between the values of the pure metal nitrides.10 Titanium vanadium nitride (Ti⫺V⫺N) coatings represent another example for the superior performance of ternary metal nitrides, as they show excellent hardness and friction properties compared to pure titanium nitride (TiN) or vanadium nitride (VN) coatings.11,12 Moreover, small amounts of vanadium in a titanium nitride should www.acsnano.org
Synthesis of Ternary Metal Nitride Nanoparticles Using Mesoporous Carbon Nitride as Reactive Template
ABSTRACT Mesoporous graphitic carbon nitride was used as both a nanoreactor and a reactant for the
synthesis of ternary metal nitride nanoparticles. By infiltration of a mixture of two metal precursors into mesoporous carbon nitride, the pores act first as a nanoconfinement, generating amorphous mixed oxide nanoparticles. During heating and decomposition, the carbon nitride second acts as reactant or, more precisely, as a nitrogen source, which converts the preformed mixed oxide nanoparticles into the corresponding nitride (reactive templating). Using this approach, ternary metal nitride particles with diameters smaller 10 nm composed of aluminum gallium nitride (AlⴚGaⴚN) and titanium vanadium nitride (TiⴚVⴚN) were synthesized. Due to the confinement effect of the carbon nitride matrix, the composition of the resulting metal nitride can be easily adjusted by changing the concentration of the preceding precursor solution. Thus, ternary metal nitride nanoparticles with continuously adjustable metal composition can be produced. KEYWORDS: nanoparticles · template · carbon nitride · metal nitride · mesoporous · semiconductor · catalysis
stabilize this material in applications such as electrodes for supercapacitors.13 These examples show that a general and facile approach, combining control over composition and nanostructure of ternary nitrides in one step, would be certainly beneficial. In general, ternary metal nitrides can be prepared by heating the respective ternary oxide precursor with nitrogen donors such as ammonia or urea.14⫺16 Also, solid state metathesis reactions using for example Li3N or NaN3 have been reported.17⫺21 However, the synthesis of defined nanostructured ternary metal nitrides is so far just rarely described (except for ternary III nitrides, especially InGaN, where several nanostructures were reported using vapor deposition22⫺24 or precursor route25,26 techniques). The synthesis of a high surface area V⫺Mo⫺N powder was achieved using nitridation of amine intercalated ternary oxide foams in a high temperature ammonia flow.27 Herein we report on the synthesis of ternary metal nitride nanoparticles using a
*Address correspondence to [email protected]
Received for review August 7, 2008 and accepted October 21, 2008. Published online November 12, 2008. 10.1021/nn800503a CCC: $40.75 © 2008 American Chemical Society
VOL. 2 ▪ NO. 12 ▪ 2489–2496 ▪ 2008
“reactive hard templating” approach, exemplified by the synthesis of Al⫺Ga⫺N and Ti⫺V⫺N nanoparticles. “Hard templating”, using mainly inorganic nanostructures as endo- or exotemplate,28 is widely applied for the synthesis of mesoporous polymers, carbon nitrides, and carbon materials.29,30 After removal of the hard template, the resulting material is often in fact an inverse replica of the initial template. Consequently, repeated hard templating procedures,31 including two successive replications steps, yield in direct copies, exhibiting ideally a similar nanostructure as observed in the initially used template. In the approach presented here, termed reactive templating, the template acts additionally as reactant, thus determining not only the structure but also the chemical composition of the resulting material. Recently, we reported on the synthesis of binary metal nitride nanoparticles using such a reactive templating.32 A mesoporous carbon nitride synthesized with silica nanoparticles as template33 were first used as exotemplate for the preparation of metal oxide nanoparticles and then as a nitrogen source converting the metal oxides into the corresponding nitride. Herein we show that ternary metal nitride nanoparticles can be synthesized using mesoporous carbon nitrides as reactive hard template accordingly. Thus, a variety of nanostructured ternary nitrides (here Al⫺Ga⫺N and V⫺Ti⫺N) can be produced with the possibility to continuously tune the metal ratios in their composition.
TABLE 1. Composition of the Infiltrating Solutions for the
Synthesis of AlⴚGaⴚN and TiⴚVⴚN Nanoparticles in mpg-C3N4 (Numbers Describe the Molar Ratio of the Metals in the Initial Precursor Solutions) sample
Al/Ga mol ratio
AlGaN-0.20 AlGaN-0.72 AlGaN-1.46 sample TiVN-0.19 TiVN-0.55 TiVN-1.46
110.0 290.0 400.0 VOCl3 (mg) 170.0 400.0 800.0
730.0 530.0 360.0 TiCl4 (mg) 1000.0 800.0 600.0
2.0 2.0 2.0 EtOH (g) 2.0 2.0 2.0
0.20 0.72 1.46 V/Ti mol ratio 0.19 0.55 1.46
pores and a surface area of 220 m2/g proven by TEM, SAXS, and nitrogen sorption measurements (Figure S2⫺S4 in the Supporting Information), respectively. The synthesis of two series of ternary metal nitrides were studied, first aluminum/gallium nitrides and second titanium/vanadium nitrides. Similar synthesis routes were applied for the synthesis of nanoparticles from these precursors: Three precursor solutions with different concentrations of GaCl3 and AlCl3 or TiCl4 and VOCl3, respectively, were prepared in ethanol, and the nanoreactor (mpg-C3N4) was added to these solutions (Table 1). The infiltrated powder was collected and carefully washed with 2 mL EtOH during suction filtration, ensuring that the precursor solutions are located in the pores of the nanoreactor only. During drying of the carbon nitride/precursor composite, the formation of amorphous mixed oxide nanoparticles confined in the RESULTS AND DISCUSSION mesopores can be assumed. It has been shown that Mesoporous graphitic carbon nitride (mpg-C3N4), 33 heating of these composites in the case of pure metal was synthesized as already described. Elemental precursors yields the formation of binary metal nitride analysis of the resulting material is proving a composinanoparticles, by donating nitrogen atoms from the tion close to the ideal stochiometry. From X-ray measurements (Figure S1 in the Supporting Information), a carbon nitride nanoreactor to the preformed metal ox32 graphitic stacking in the material can be observed, indi- ide nanoparticles. The same mechanism can be assumed for precurcated by a peak at 27.5°, which can be indexed accordsor mixtures confined in the mesopores of mpg-C3N4, ing to the (002) peak from a graphitic structure while with the advantage that a possible demixing or phase the peak at 13.1° can be attributed to an in-plane periseparation of the different metals is prevented as long odic order.34 The mpg-C3N4 used in this study as reacas the nanoconfinement is present. In the following, the tive template features interconnected 12 nm spherical synthesis of aluminum gallium nitrides and titanium vanadium nitrides are discussed separately. Synthesis of AlⴚGaⴚN Nanoparticles in Mesoporous Graphitic Carbon Nitride. Solutions of AlCl3 and GaCl3 in ethanol with different Al/Ga molar ratios were used as precursors and infiltrated into mpg-C3N4 (see Table 1). To define the boundary cases, pure AlCl3 and GaCl3 solutions were used, which yield in the formation of the pure, binary nitrides. The infiltrated mpg-C3N4 powders were heated to 800 °C under nitrogen flow, as described for the synthesis of pure GaN nanoparticles.32 It should be noted that the Figure 1. EDX measurements of the AlⴚGaⴚN nanoparticles: (a) AlGaN-0.20, (b) AlGaNreaction can be also carried out under argon 0.72, and (c) AlGaN-1.46. 2490
VOL. 2 ▪ NO. 12 ▪ FISCHER ET AL.
Analysis (N,C): For Comparison, the Initial Molar Ratios of the Metals in the Precursor Solution Are Also Shown sample
Al wt %
Ga wt %
N wt %
C wt %
O wt %
residue wt %
molar ratio Al/Ga (powder)
molar ratioAl/Ga (solution)
AlGaN-0.20 AlGaN-0.72 AlGaN-1.46
6.41 19.20 28.68
73.81 62.46 52.03
15.28 15.17 15.02
0.00 0.00 0.00
0.76 1.20 0.88
3.74 1.83 3.39
0.22 0.79 1.42
0.20 0.72 1.46
or in sealed quartz ampoules, proving that the TABLE 3. Cell Parameters and Crystallite Size of the nitrogen is provided by the C3N4 template. A higher Observed AlⴚGaⴚN, GaN, and AlN Powders Synthesized temperature than the decomposition temperature of in the Same Reaction Conditions mpg-C3N4 (⬃650 °C) was used, as this temperature cell parameter [Å] P63mc should ensure complete removal of the template. After a c cryst size XRD particle size TEM the samples were completely cooled to room tempera- sample ture under nitrogen atmosphere, powders from light GaN 3.189 5.184 9.1 9.0 yellow-brown to light gray in color were obtained (with AlGaN-0.20 3.179 5.16 9.6 9.2 AlGaN-0.72 3.173 5.138 7.5 7.4 increasing amount of aluminum). The composition of 3.165 5.105 5.9 4.2 the powders was determined using electron dispersive AlGaN-1.46 AlN 3.112 4.975 9.5 11 X-ray spectroscopy (EDX) and elemental analysis. The EDX measurements in Figure 1 illustrate the increasing minum content, a decrease in the crystal size from 9.6 aluminum content of the resulting powders, following to 5.9 nm is observed in the ternary samples, while the the increasing amount of aluminum in the preceding binary metal nitrides show a similar crystallite size of apprecursor mixtures. Table 2 summarizes the composition of the powders determined by EDX. It can be seen proximately 9 nm. However, it should be noted that, although the broadness of the reflection peaks is related that the molar ratios of the initial precursor solutions to the crystal size, also the quality of the crystal strucare nearly perfectly reflected in the resulting metal 35 nitrides. The nitrogen content of the samples was addi- ture can have a significant influence. Thus, progressive peak broadening could also reflect a loss in crystaltionally confirmed by elemental analysis. For all three linity due to an increasing number of defects when samples, the amount of nitrogen found is approxithe aluminum content is increased. However, in the mately 15 wt %, which is in good agreement with the EDX determined values. Only traces of oxygen could be detected, indicating that only minor surface oxidation on the nanoparticles occurs. Remarkably, no carbon contamination is found in the powders, which is confirmed both by EA and EDX. Powder X-ray diffraction measurements (PXRD) (Figure 2) show that all powders feature hexagonal symmetry and crystallize in the space group P63mc, according to a solid solution of GaN and AlN. Comparing these patterns with the reflections found for pure gallium and aluminum nitride, a significant shift in the pattern of the powders from lower angles, that is, from pure GaN, to higher angles toward pure AlN is observed with increasing aluminum content in the powders (Figure 2). This shift indicates the formation of a solid solution, thus aluminum atoms progressively substitute gallium atoms in the crystal. The cell parameters for each sample and those of pure GaN and AlN are listed in Table 3. The Scherrer equation was applied to the (102) and the (110) peaks to determine an average crystal size for each sample. The most intensive peak, Figure 2. Powder X-ray diffraction pattern of the AlⴚGaⴚN nanocrystalline namely, the (101) peak, could not be used to powders with increasing aluminum content: (a) AlGaN-0.20, (b) AlGaN-0.72, and determine the crystallite size since it overlaps (c) AlGaN-1.46. As a reference, the patterns of pure GaN and AlN synthesized in with the adjacent (002) peak. With increasing alu- the same conditions are also shown. www.acsnano.org
VOL. 2 ▪ NO. 12 ▪ 2489–2496 ▪ 2008
TABLE 2. Composition of the Different AlⴚGaⴚN Nanocrystalline Powders Determined by EDX (Al,Ga, O) and Elemental
of well-developed lattice fringes. To ensure an accurate comparison between the lattice distances in the three samples, just particles oriented along the  zone axis were chosen for measurements. The measured lattice distances for the samples AlGaN-0.20, AlGaN-0.72, and AlGaN-1.46 were 2.74, 2.73, and 2.71 Å, respectively (Figure S5 Figure 3. TEM micrographs of the AlⴚGaⴚN samples: (a) AlGaN-0.20, (b) AlGaN-0.72, and (c) AlGaN-1.46. The powders were dispersed in THF using oleic acid prior to the measurements. in the Supporting Information). These distances do not perfectly fit with the d100 lattice distances measured by XRD case of the AlGaN-1.46 sample, a small shoulder at (Table 2) but at least follow the observed trend, namely, higher angles is present in the (102) peak. Thus, it is that the lattice distances decrease with increasing alulikely that a component with a higher Al content, and minum content. This confirms on the nanometer scale thus smaller lattice parameters (shoulder), coexists with the formation of an Al⫺Ga⫺N solid solution in the form the major phase (main (102) peak). of nanoparticles, formed from the preceding mixed soThe size and shape of the particles were investilutions confined in the mesopores of the nitrogen dogated by transmission electron microscopy (TEM). The nor, namely, mpg-C3N4. TEM measurements (Figure 3) of dispersed samples It can be concluded that mesoporous carbon nishow that the powders consist of small nanoparticles tride is indeed a suitable nanoreactor for the synthesis with a narrow dispersity, confirming the results obof pure Al⫺Ga⫺N nanoparticles with dimensions less tained from the X-ray diffraction and supporting the than 10 nm. Furthermore, it was shown that the compoconcept that nanoparticles are formed through the consition of the alloy nanoparticles could be continuously finement by the mesopores of the carbon nitride. The adjusted in the experimental range explored here by average particle size determined from the TEM pictures simply changing the Al/Ga ratio in the precursor (see Table 2) correlates with small deviations with the solution. crystallite size determined from the Scherrer equation. Synthesis of TiⴚVⴚN Nanoparticles in Mesoporous Graphitic The particle sizes derived from XRD and TEM are Carbon Nitride. To prove the versatility of the approach smaller than the pore size of the initial template, mpgshown here, the concept was expanded to the preparaC3N4, which features a pore of 12 nm in diameter. This tion of nanoparticles from a second ternary metal nican also be expected as the metal precursors are intro- tride, namely, titanium vanadium nitride. Here, soluduced as solutions in the nanoconfinement, thus they tions of TiCl4 and VOCl3 in ethanol with different Ti/V are not able to completely fill out the pore. In a recent molar ratios were used as precursors and infiltrated into paper, it has been shown that indeed the concentration mpg-C N (see Table 1). Pure TiCl or VOCl solutions 3 4 4 3 of the precursor solution can be used to tune the size were used to prepare also the pure binary metal nitrides 32 of the resulting nanoparticles. as boundary cases. The infiltrated mpg-C3N4 powders In Figure 4, a complementary HRTEM measurement were heated to 800 °C under nitrogen flow, as deis shown. The powders consist of highly crystalline, ag- scribed for the synthesis of pure TiN or VN nanopartiglomerated nanoparticles, as depicted by the presence cles.32 After the samples were completely cooled to room temperature under nitrogen atmosphere, black powders were observed in all cases. The composition of the powders was investigated as described for Al⫺Ga⫺N nanoparticles. The EDX (Figure 5) measurements of the powders show the increasing vanadium content following the concentrations in the preceding precursor solution. However, contrary to the Al⫺Ga⫺N nanoparticles where no residual carbon was observed, for Ti⫺V⫺N samples, large amounts of carbon are detected (Table 4). This is not surprising since similar observations were made for mesoporous TiN8 and TiN nanoparticles36 synthesized with carbon nitride (or cyanamide) as nitrogen source. Furthermore, the amount of oxygen found in the samples is higher than in the case of the AlxGa1⫺xN samples, thus some amount of surface oxiFigure 4. HRTEM micrograph of the sample AlGaN-1.46. The inset shows the dation has to be taken into account. Nevertheless, the indexed FFT of the area delimited with the red circle. VOL. 2 ▪ NO. 12 ▪ FISCHER ET AL.
Comparison, the Initial Molar Ratios of the Metals in the Precursor Solution Are Also Shown sample
V wt %
Ti wt %
N wt %
C wt %
O wt %
residue wt %
molar ratio V/Ti (powder)
molar ratio V/Ti (solution)
TiVN-0.19 TiVN-0.55 TiVN-1.46
4.50 8.90 14.02
22.01 15.00 8.91
11.19 11.60 9.60
51.78 53.14 55.6 1
6.02 6.03 5.94
4.51 5.33 5.95
0.19 0.56 1.48
0.19 0.55 1.46
presence of larger amounts of titanium oxide or vanadium oxide in the samples can be excluded as shown by the absence of reflection patterns corresponding to the respective oxides in the XRD measurements (Figure 6). On the other hand, an incorporation of oxygen inside the crystal structure cannot be excluded since for both compounds Ti(ON)37,38 and V(ON)39 phases are known and inclusion of small amounts of oxygen should not change the XRD pattern significantly. All three samples exhibit diffraction patterns with cubic symmetry and crystallize in the space group Fm3¯m. The exact peak positions as well as the cell parameters are listed in Figure 5. EDX measurements of the TiⴚVⴚN nanoparticles: (a) TiVN-0.19, (b) TiVNTable 5. As observed for the Al⫺Ga⫺N nano0.55, and (c) TiVN-1.46. particles, a shift in the diffraction angles is observed depending on the Ti/V molar ratio in the powders. Thus, with increasing vanadium content, the pattern shifts to higher angles, that is, from the pattern of pure TiN toward the pattern of pure VN, indicating the formation of a homogeneous Ti⫺V⫺N solid solution. From the Scherer equation applied to the (200) and the (111) peak, an average crystallite size was determined for each sample. The crystallite size decreases from 5.0 to 3.7 nm with increasing vanadium content, indicated by a progressive broadening of the diffraction peaks. In contrast, the crystallite size of the two binary Figure 6. X-ray diffraction pattern of the TiⴚVⴚN powders nitrides is similar at approximately 5 nm. with increasing vanadium content: (a) TiVN-0.19, (b) TiVNThe shape and size of the particles were further0.55, and (c) TiVN-1.46. As a reference, the patterns of pure TiN and VN synthesized in the same reaction conditions are more investigated by TEM measurements (Figure 7). The TEM images show small particles of narrow disper- shown. sity, which are, contrary to the Al⫺Ga⫺N particles, not sidual carbon causes significant background noise in isolated but embedded in an amorphous matrix, most the FFT. Still a trend toward smaller lattice distances probably formed from the residual carbon. The higher with increasing vanadium content is observed. agglomeration and thus higher density of the particles enables additional confirmation of the crystallinity of the samples using selected area electron diffraction TABLE 5. Diffraction Peak Positions, Cell Parameters, and (SAED). The observed SAED patterns can be attributed Crystallite Size of the Observed TiⴚVⴚN, TiN, and VN to Ti⫺V⫺N alloys. Powders Synthesized in the Same Reaction Conditions HRTEM measurements show that the particles are cell parameter [Å] Fm3¯m highly crystalline, and well-developed lattice fringes sample aⴝbⴝc cryst size XRD particle size TEM can be observed (Figure 8). From the corresponding TiN 4.233 4.8 5.6 FFT, the lattice distances were determined. However, TiVN-0.19 4.220 5.0 5.0 TiVN-0.55 4.205 4.6 5.0 particles with similar orientations were harder to find 4.160 3.7 4.0 in these samples, making an accurate comparison of the TiVN-1.46 4.130 4.9 5.5 lattice distances difficult. Moreover, the presence of re- VN www.acsnano.org
VOL. 2 ▪ NO. 12 ▪ 2489–2496 ▪ 2008
TABLE 4. Composition Determined by EDX (Ti,V, O) and Elemental Analysis (C,N) of the Different TiⴚVⴚN Powders: For
as reactant for the conversion of the oxide into the nitride. Using this approach, ternary metal nitride nanoparticles with particle sizes smaller than 10 nm, narrow dispersities, and controlled composition could be synthesized, here exemplified by the synthesis of Al⫺Ga⫺N and Ti⫺V⫺N nanoparticles, respectively. EDX measurements revealed that Figure 7. TEM micrographs and SAED of the TiⴚVⴚN samples: (a) TiVN-0.19, (b) TiVN-0.55, the composition of the final nitrides is and (c) TiVN-1.46. simply dependent on the prior used precursor ratios, while XRD and HRTEM proved that indeed homogeneous, solid solutions of the two metal nitrides have formed also on the scale of one single nanoparticle. From these examples, it can be assumed that the reactive templating shown here is a quite general approach, which could be used for the preparation of nanoparticles with a wide variety of other ternary metal nitride compositions. Furthermore, as the nanoconfinement prevents any phase separation or demixing of the metals, there seems to be no borderline to the used metal compositions, and even the generation of quaternary and higher metal nitrides can be envisaged. Also, as the size of the nanoparticles can be tuned by simply changing the concentration of the preceding solutions,32 not only the composition but also the size of the nanoparticles should be easily adjustable. Thus we think that the reactive templating shown here can certainly complement other metal nitride syntheses, such as post-treatment of mixed oxides with nitrogen donors such as ammonia. Nanoparticles are presumably the most often described nanostructure of inorganic Figure 8. HRTEM micrographs and FFT spectrum of the TiⴚVⴚN samples: (a) TiVNmaterials. However, it should be noted that for 0.19, (b) TiVN-0.55, and (c) TiVN-1.46. this conceptual paper we restricted ourselves to CONCLUSION the simplest topology of the reactive template, a mesoIn conclusion, mesoporous graphitic carbon nitride porous carbon nitride with spherical pores produced (mpg-C3N4) was used as a “reactive template” for the by templating silica nanoparticles. The ternary metal nisynthesis of ternary metal nitride nanoparticles. Infiltratride particles produced here are therefore in the end tion of solutions of mixed precursors and removal of just a direct copy of the morphology of the initially used the solvent yield the formation of mixed metal oxide silica nanoparticles. Considering the abundance of nanoparticles in the pores. Subsequent heating under inert gas yields decomposition of the metal nitride and other silica nanostructures available, from particles to the donation of nitrogen atoms to the preformed oxide porous materials, a variety of other morphologies in which ternary metal nitrides can be shaped can be nanoparticles. Thus, in the first step, mpg-C3N4 acts as a classical exotemplate, while in the second step, it acts envisaged using the approach shown here.
METHODS All chemicals were used as received without any further purification. Synthesis of Mesoporous C3N4. The nanoreactor, mpg-C3N4, was synthesized as previously described.33 In a typical synthesis,
VOL. 2 ▪ NO. 12 ▪ FISCHER ET AL.
2.5 g of a 40 wt % aqueous silica nanoparticle solution (Ludox HS40, Ø ⬃ 12 nm, Aldrich) was added to 1 g of molten cyanamide (CH2N2, Aldrich). The mixture was then heated to 90 °C under vigorous stirring to ensure the slow evaporation of the water. The resulting white solid was heated in a closed ceramic crucible to 550 °C for 4 h. Removal of the silica nanoparticles with
Acknowledgment. Financial support by the Max Planck Society within the framework of the project ENERCHEM is gratefully acknowledged. Supporting Information Available: Analysis (XRD, TEM, SAXS, BET) of the reactive template, mpg-C3N4, diffraction peak positions of the Al⫺Ga⫺N and Ti⫺V⫺N, and additional HRTEM micrographs for Al⫺Ga⫺N nanoparticles are reported. This material is available free of charge via the Internet at http:// pubs.acs.org.
REFERENCES AND NOTES 1. Sirvio, E. H.; Sulonen, M.; Sundquist, H. Abrasive Wear of Ion-Plated Titanium Nitride Coatings on Plasma-Nitrided Steel Surfaces. Thin Solid Films 1982, 96, 93–101. 2. Ponce, F. A.; Bour, D. P. Nitride-Based Semiconductors for Blue and Green Light-Emitting Devices. Nature 1997, 386, 351–359. 3. Choi, D.; Blomgren, G. E.; Kumta, P. N. Fast and Reversible Surface Redox Reaction in Nanocrystalline Vanadium Nitride Supercapacitors. Adv. Mater. 2006, 18, 1178–1182. 4. Krawiec, P.; De Cola, P. L.; Glaser, R.; Weitkamp, J.; Weidenthaler, C.; Kaskel, S. Oxide Foams for the Synthesis of High-Surface-Area Vanadium Nitride Catalysts. Adv. Mater. 2006, 18, 505–508.
5. Kaskel, S.; Schlichte, K.; Kratzke, T. Catalytic Properties of High Surface Area Titanium Nitride Materials. J. Mol. Catal. A: Chem. 2004, 208, 291–298. 6. Kwon, H.; Choi, S.; Thompson, L. T. Vanadium Nitride Catalysts: Synthesis and Evaluation for n-Butane Dehydrogenation. J. Catal. 1999, 184, 236–246. 7. Ramanathan, S.; Oyama, S. T. New Catalysts for HydroprocessingOTransition-Metal Carbides and Nitrides. J. Phys. Chem. 1995, 99, 16365–16372. 8. Fischer, A.; Makowski, P.; Mu¨ller, J. O.; Antonietti, M.; Thomas, A.; Goettmann, F. High-Surface-Area TiO2 and TiN as Catalysts for the C⫺C Coupling of Alcohols and Ketones. ChemSusChem 2008, 1, 444–449. 9. Jain, S. C.; Willander, M.; Narayan, J.; Van Overstraeten, R. III-Nitrides: Growth, Characterization, and Properties. J. Appl. Phys. 2000, 87, 965–1006. 10. Benaissa, M.; Gonsalves, K. E.; Rangarajan, S. P. AlGaN Nanoparticle/Polymer Composite: Synthesis, Optical, and Structural Characterization. Appl. Phys. Lett. 1997, 71, 3685–3687. 11. Latella, B. A.; Gan, B. K.; Daviesb, K. E.; McKenzie, D. R.; McCulloch, D. G. Titanium Nitride/Vanadium Nitride Alloy Coatings: Mechanical Properties and Adhesion Characteristics. Surf. Coat. Technol. 2006, 200, 3605–3611. 12. Ichimiya, N.; Onishi, Y.; Tanaka, Y. Properties and Cutting Performance of (Ti,V)N Coatings Prepared by Cathodic Arc Ion Plating. Surf. Coat. Technol. 2005, 200, 1377–1382. 13. Choi, D.; Kumta, P. N. Nanocrystalline TiN Derived by a Two-Step Halide Approach for Electrochemical Capacitors. J. Electrochem. Soc. 2006, 153, A2298–A2303. 14. Herle, P. S.; Vasanthacharya, N. Y.; Hegde, M. S.; Gopalakrishnan, J. Synthesis of New Transition-Metal Nitrides, MWN2 (M ⫽ Mn, Co, Ni). J. Alloys Compd. 1995, 217, 22–24. 15. Bem, D. S.; Loye, H. C. Z. Synthesis of the New Ternary Transition-Metal Nitride FeWN2 via Ammonolysis of a Solid State Precursor. J. Solid State Chem. 1993, 104, 467– 469. 16. Gomathi, A. Ternary Metal Nitrides by the Urea Route. Mater. Res. Bull. 2007, 42, 870–874. 17. Parkin, I. P. Solid State Metathesis Reaction for Metal Borides, Silicides, Pnictides and Chalcogenides: Ionic or Elemental Pathways. Chem. Soc. Rev. 1996, 25, 199–207. 18. Parkin, I. P.; Nartowski, A. M. Solid State Metathesis Routes to Group IIIa Nitrides: Comparison of Li3N, NaN3, Ca3N2 and Mg3N2 as Nitriding Agents. Polyhedron 1998, 17, 2617–2622. 19. Cumberland, R. W.; Blair, R. G.; Wallace, C. H.; Reynolds, T. K.; Kaner, R. B. Thermal Control of Metathesis Reactions Producing GaN and InN. J. Phys. Chem. B 2001, 105, 11922–11927. 20. Gillan, E. G.; Kaner, R. B. Rapid Solid-State Synthesis of Refractory Nitrides. Inorg. Chem. 1994, 33, 5693–5700. 21. Song, B.; Jian, J. K.; Wang, G.; Lei, M.; Xu, Y. P.; Chen, X. L. Facile and General Route to Nitrides by a Modified SolidState Metathesis Pathway. Chem. Mater. 2007, 19, 1497–1502. 22. Hsu, C. W.; Ganguly, A.; Liang, C. H.; Hung, Y. T.; Wu, C. T.; Hsu, G. M.; Chen, Y. F.; Chen, C. C.; Chen, K. H.; Chen, L. C. Enhanced Emission of (In, Ga) Nitride Nanowires Embedded with Self-Assembled Quantum Dots. Adv. Funct. Mater. 2008, 18, 938–942. 23. Cai, X. M.; Leung, Y. H.; Cheung, K. Y.; Tam, K. H.; Djurisic, A. B.; Xie, M. H.; Chen, H. Y.; Gwo, S. Straight and Helical InGaN Core-Shell Nanowires with a High In Core Content. Nanotechnology 2006, 17, 2330–2333. 24. He, M. Q.; Mohammad, S. N. Novel Chemical-Vapor Deposition Technique for the Synthesis of High-Quality Single-Crystal Nanowires and Nanotubes. J. Chem. Phys. 2006, 124, 064714-1–064714-7. 25. Bhat, S. V.; Biswas, K.; Rao, C. N. R. Synthesis and Optical Properties of In-Doped GaN Nanocrystals. Solid State Commun. 2007, 141, 325–328.
VOL. 2 ▪ NO. 12 ▪ 2489–2496 ▪ 2008
a 4 M NH4HF2 solution yielded mesoporous graphitic carbon nitride (mpg-C3N4). Caution is advised as NH4HF2 causes severe burns in contact with skin. Synthesis of Metal Nitride Alloy Nanoparticles AⴚBⴚN. In a general synthesis, the respective amount of precursors A and B was dissolved in 2.0 g of ethanol. Caution is advised because the described metal precursors (GaCl3, AlCl3, TiCl4, and VOCl3) react vigorously with ethanol. Transparent solutions were obtained in all cases. The exact composition of the used precursor solutions is given in Table 1. To these solutions was added 0.5 g of mesoporous g-C3N4. The mixtures were sonicated for 10 min and placed shortly under reduced pressure to free the pores from air and thus to achieve a good penetration of the solution inside the pores. The infiltrated mesoporous powder was collected by suction filtration washed dropwise under suction with 2 mL of EtOH, and finally dried on the filter. The resulting powder was heated to 800 °C for 4 h and kept there for 3 h, both under a flow of nitrogen. Caution is advised as the thermal decomposition of C3N4 can yield the production of toxic gases such as HCN. Thus, ovens have to be placed in a fume hood or places with sufficient ventilation. After the heat treatment, light brown to gray powders for Al⫺Ga⫺N and black powders for Ti⫺V⫺N were obtained, respectively. Characterization. TEM images were taken on a Zeiss EM Omega 912X at an acceleration voltage of 120 kV. The as-made powders were grinded and dispersed in acetone or THF. One droplet of oleic acid was added, and the suspension was strongly sonicated several times with a high power sonicating tip to ensure better dispersion of the particles. One droplet of the suspension was applied to a 400 mesh carbon-coated copper grid and left to dry. HRTEM images of the Al⫺Ga⫺N particles were performed on a Phillips TEM/STEM CM 200 FEG transmission electron microscope equipped with a field-emission gun operated at 200 kV. HRTEM images of the Ti⫺V⫺N samples were conducted with a JEOL TEM/STEM JEM-2100F-UHR transmission electron microscope equipped with a field-emission gun operated at 200 kV. XRD measurements were carried out in reflection mode on a Bruker D8 diffractometer. The emitted Cu K␣ radiation ( ⫽ 0.154 nm) was monochromated by a multilayer Go¨bel mirror. An energy dispersive detector (Sol-X, Bruker) was used to ensure low background noise, by filtering out the inelastic scattered photons. SEM measurements were carried out on a DSM 940 A microscope from Zeiss (Oberkochen), which operates at 20 kV. For EDX measurements, a Link-ISIS 300 from Oxford Instruments (UK) was used. Elemental analyses were performed with a VARIO EL elemental analysis instrument to determine the carbon, nitrogen, hydrogen, and sulfur content of the samples.
26. Schwenzer, B.; Meier, C.; Masala, O.; Seshadri, R.; DenBaars, S. P.; Mishra, U. K. Synthesis of Luminescing (In, Ga)N Nanoparticles from an Inorganic Ammonium Fluoride Precursor. J. Mater. Chem. 2005, 15, 1891–1895. 27. Krawiec, P.; Panda, R. N.; Kockrick, E.; Geiger, D.; Kaskel, S. High Surface Area V-Mo-N Materials Synthesized from Amine Intercalated Foams. J. Solid State Chem. 2008, 181, 935–942. 28. Schuth, F. Endo- and Exotemplating to Create HighSurface-Area Inorganic Materials. Angew. Chem., Int. Ed. 2003, 42, 3604–3622. 29. Lu, A. H.; Schuth, F. Nanocasting: A Versatile Strategy for Creating Nanostructured Porous Materials. Adv. Mater. 2006, 18, 1793–1805. 30. Thomas, A.; Goettmann, F.; Antonietti, M. Hard Templates for Soft Materials: Creating Nanostructured Organic Materials. Chem. Mater. 2008, 20, 738–755. 31. Tiemann, M. Repeated Templating. Chem. Mater. 2008, 20, 961–971. 32. Fischer, A.; Antonietti, M.; Thomas, A. Growth Confined by the Nitrogen Source: Synthesis of Pure Metal Nitride Nanoparticles in Mesoporous Graphitic Carbon Nitride. Adv. Mater. 2007, 19, 264–267. 33. Goettmann, F.; Fischer, A.; Antonietti, M.; Thomas, A. Chemical Synthesis of Mesoporous Carbon Nitrides Using Hard Templates and Their Use as a Metal-Free Catalyst for Friedel⫺Crafts Reaction of Benzene. Angew. Chem., Int. Ed. 2006, 45, 4467–4471. 34. Thomas, A.; Fischer, A.; Goettmann, F.; Antonietti, M.; Muller, J.-O.; Schlogl, R.; Carlsson, J. M. Graphitic Carbon Nitride Materials: Variation of Structure and Morphology and Their Use as Metal-Free Catalysts. J. Mater. Chem. 2008, 18, 4893–4908. 35. Stutzmann, M.; Ambacher, O.; Cros, A.; Brandt, M. S.; Angerer, H.; Dimitrov, R.; Reinacher, N.; Metzger, T.; Hopler, R.; Brunner, D.; et al. Properties and Applications of MBE Grown AlGaN. Mater. Sci. Eng., B 1997, 50, 212–218. 36. Buha, J.; Djerdj, I.; Antonietti, M.; Niederberger, M. Thermal Transformation of Metal Oxide Nanoparticles into Nanocrystalline Metal Nitrides Using Cyanamide and Urea as Nitrogen Source. Chem. Mater. 2007, 19, 3499–3505. 37. Hitoki, G.; Takata, T.; Kondo, J. N.; Hara, M.; Kobayashi, H.; Domen, K. (Oxy)nitrides as New Photocatalysts for Water Splitting under Visible Light Irradiation. Electrochemistry 2002, 70, 463–465. 38. Martinez-Ferrero, E.; Sakatani, Y.; Boissiere, C.; Grosso, D.; Fuertes, A.; Fraxedas, J.; Sanchez, C. Nanostructured Titanium Oxynitride Porous Thin Films as Efficient VisibleActive Photocatalysts. Adv. Funct. Mater. 2007, 17, 3348–3354. 39. Parkin, I. P.; Elwin, G. S. Atmospheric Pressure Chemical Vapour Deposition of Vanadium Nitride and Oxynitride Films on Glass from Reaction of VCl4 with NH3. J. Mater. Chem. 2001, 11, 3120–3124.
VOL. 2 ▪ NO. 12 ▪ FISCHER ET AL.